Faculty of Physics, Shahid Bahonar University of Kerman, Kerman, Iran
Faculty of Physics, Shahid Bahonar University of Kerman, Kerman, Iran
Faculty of Physics, Shahid Bahonar University of Kerman, Kerman, Iran
^{} Faculty of Physics, Shahid Bahonar University of Kerman, Kerman, Iran
Magnetic Materials Advances 2018, 1, 1–4. doi:10.26705/magmatadv.2018.1.1.1-4
Received 09 May 2018,
Accepted 04 June 2018,
Published 04 June 2018
Herein, we report the potential of polar bi-gyrotropic single-negative magnetic metamaterials (that their ε and μ are in the form of non-diagonal tensors) to act simultaneously as reflector and magnetic rotator layer. In other word, we report the development of the single-negative metamaterials at a prominent location in magneto-optics. To understand the optical and magneto-optical properties of polar bi-gyrotropic single-negative layers, we have firstly introduced a transfer matrix method (TMM) based-approach and then we have numerically studied the propagation of electromagnetic wave through such medium. The study of the electromagnetic wave propagation through the polar bi-gyrotropic single-negative material may help to study the unusual behavior of the MO periodic structures (such as magnetophotonic crystals) containing them. The study exposes that such polar bi-gyrotropic single-negative layers can be used to make controlled and to enhance the optical and MO properties of optical.
Keywords: Bi-gyrotropic magnetic medium, Single-negative metamaterial, Polar magnetization, Transfer matrix method.
Metamaterials are artificial materials and engineered composites in which their electromagnetic properties (ε and μ) can be controlled, because, they make possible the manipulation of fields and waves at subwavelength scales. Advances in simulation and fabrication technologies have brought about broad flexibilities in the design of metamaterials and, consequently, their electromagnetic responses with super performances [1-4]. Single-negative (SNG) materials are two kinds of metamaterials: The ε -negative (ENG) material with ε < 0 while μ > 0, and the μ-negative (MNG) material with ε > 0 while μ < 0. They have significant applications in perfect lens, flat lens imaging and light trapping [5-7].
The SNG materials usually due to including plasmonic or ferromagnetic materials ingle-negative materials have intrinsic optical anisotropy properties [8-10]. On the other hand, many commonly used metamaterial structures exhibit magneto-electric coupling, hence, such media are represented as bi- anisotropic [11-13].
Optical anisotropy of a magnetic material can be seen in the light reflection from material surface and when light passes through the magnetic layers. Among MO effects, magneto-optical polar effect demonstrates itself by variation of light polarization for and longitudinal magnetization when both magnetization and propagation vectors are parallel and perpendicular to the interface [14-15]. This MO effect may be simultaneously described by nonzero off-diagonal ε and μ tensors, so that the related material is known as a bi-gyrotropic material [15].
In this paper, we have firstly provided a general framework for using the polar bi-gyrotropic single-negative magnetic materials in multilayer structures. The optical and MO properties of such structures are generally calculated by transfer matrix method (TMM). Therefore, a 4×4 TMM approach has been introduced to evaluate such multilayer structures including bi-gyrotropic SNG magnetic materials in polar magnetization configuration. Finally, by using this universal approach, to investigate the potential of reflectance and magneto-optical Kerr rotation performances of polar bi-gyrotropic single-negative magnetic materials, numerical computations have been carried out.
For the purpose of using the potential of bi-gyrotropic SNG materials in multilayer structures, transfer matrix method which can apply bi-gyrotropic SNG materials should be employed. In order to do so, we attempted to generalize the transfer matrix method introduced by Zak et al [16] to bi- gyrotropic SNG materials and propose an approach related to them. The above-mentioned approach and the others introduced by us [17-20] can be applied to structures containing bi-, single- and non-gyrotropic as well as positive and negative materials.
This method is based on definition of two 4×4 matrices: one is boundary matrix and the other propagation matrix related to each layer, which both are directly adopted for applying boundary conditions to the problem. The boundary matrix relates the tangential components of the electric and magnetic fields to the s and p components of the electric field, while the second matrix (medium propagation matrix), relates the s and p components of the electric field to the two surfaces of each layer or at any point inside the layers. Total transfer matrix in a multilayer system is obtained by multiplying matrices related to all layers. This matrix presents optical and magneto-optic features of the structure.
To simplify the use of TMM method, components of electric field corresponding to s and p polarizations are applied. Therefore, other set of fields as E_{s}^{(i)} , E_{p}^{(i)} , E_{s}^{(r)} and E_{p}^{(r)} are applied; so that s and p denote components of electric field perpendicular to or parallel with the incident plane, respectively. Moreover, the indices i and r refer to incident and reflective components of light beam, respectively. Tangential components of electric (E_{x} and E_{y} ) and magnetic (H_{x} and H_{y} ) fields are presented in the form of column matrix of F and s and p components of electric field in the form of column matrix of P, as follows. Obtaining MO coefficients, we require a matrix relating the components of two matrices of F, and P, which we call it the boundary matrix A of the medium.
Obtaining the medium boundary matrix for a bi-gyrotropic SNG magnetic medium is the main purpose of the present approach, which can be easily generalized to non-magnetic and single-gyrotropic SNG media. Here, it is attempted to present our considered approach for specific state of polar magnetization in which magnetization vector is oriented perpendicularly to the interface. For a bi-gyrotropic ENG and MNG magnetic medium, electric permittivity tensor (ε) and magnetic permeability (μ) of a medium for polar magnetization configuration are as follows,
in which, in these equations, −ε_{1} and μ_{1} form the bi-gyrotropic ENG medium, while ε_{1} and −μ_{1} form the bi-gyrotropic MNG medium. On the other hand, ε_{2} and μ_{2} are magnetic rotation parameters which have a linear relationship with magnetization vector. Furthermore, Q_{E} and Q_{M} are electric and magnetic magneto-optic constants, respectively.
To obtain the boundary and propagation matrices, in spite of the difference in details, the reader can follow a similar framework with ref [17,18]. According to the equation D = ε⃡ E and that in the local coordinate system D_{z′} = 0, we can derive the relation between x and y’ components of the D- wave for all components of the beams 1, 2, 3, and 4 (where the indices 1 and 2 are dealing with forward waves, while 3 and 4 denote backward waves inside the magnetic bi-gyrotropic medium) in both bi-gyrotropic ENG and MNG medium for specific states of polar magnetization, as follows: for the both bi-gyrotropic ENG and MNG magnetic media:
In addition, the relations between components of D in polar geometry for both bigyrotropic ENG and MNG magnetic media are as below:
in which α_{z} = cosθ_{2} and α_{y} = sinθ_{2} , so that θ_{2} is the refracted angle in the medium 2 (bi-gyrotropic SNG medium). In addition, similar relations can be acquired for 3 and 4 waves.
By using relations (2)-(7), D = ε⃡ E and D_{ z′} = 0, the relationship between the components of the electric field for the forward and backward waves in bi-gyrotropic ENG and MNG magnetic media can be obtained as:
in which N = √ε_{1}μ_{1}.
In the following, we are going to calculate the tangential components of magnetic field (H_{x} and H_{y} ) in terms of the component of the column matrix P by using the relation μ⃡ H = n × E. In this equation, n is a vector that its magnitude defines the refractive index and its direction denotes the propagation direction. Therefore, the H x and H y components of the magnetic field for the whose four waves inside the medium will be as
in which the upper (lower) signs are related to ENG (MNG) case. Also, it should be noticed that α_{z}^{(j)}= cosθ_{2}^{(j)} and α_{y}^{(j)} = sinθ_{2}^{(j)} are the cosines and sines of the angles θ_{2}^{(j)} , and j=1,2,3,4 according to four waves inside the bigyrotropic ENG and MNG magnetic medium.
By using snell’s law and Eqs. (10) and (11), the coefficients of α_{z}^{(j)} and α_{y}^{(j)} for the forward and backward waves in bi-gyrotropic ENG and MNG magnetic media in polar geometry can be obtained as follows:
By substituting the Eqs. (8)-(11) as well as Eqs. (14) and (15) in Eqs. (12) and (13), the components of magnetic field for four waves inside a bi- gyrotropic ENG and MNG medium in polar cases can be achieved. Hence, up to now, the matrix F has been obtained.
However, to derive the boundary matrix A, we also have to determine the matrix P including s and p components of electric field inside the bi- gyrotropic ENG and MNG medium. In this way, we can write the s and p components of electric field for incident and reflected waves inside the bi- gyrotropic SNG magnetic layer as
in which unit vectors of ŷ^{(i)} and ŷ^{(r)} denote the directions of axes y^{(i)} and y^{(r)} , respectively. These unit vectors are defined as
Finally, the boundary matrix A for both bi-gyrotropic ENG and MNG materials in polar geometry, according to the relation between tangential components of electric and magnetic fields and s and p components of electric field, can be obtained as follows: SNG magnetic layer as
Moreover, the propagation matrix of a bi-gyrotropic ENG and MNG magnetic medium for polar magnetization, by following the formalism of ref [16], is formed as
in which the upper (lower) sign denotes a bi-gyrotropic ENG (MNG) magnetic medium for polar magnetization; while U = exp (kNα_{z}d) and U = exp [kNd(Q_{E} + Q_{M} )/2]. In addition, d is of the thickness bi-gyrotropic SNG magnetic medium. Also, k is the wave number. It should be noted that the propagation matrix can be generalized to non-magnetic SNG materials by having the MO constants equal to zero. These matrices are the boundary and propagation matrices for bi-gyrotropic ENG and MNG magnetic media. If we set Q_{E} = 0 or Q_{M} = 0, the related matrices for a single-gyrotropic ENG and MNG magnetic medium can be achieved; and if both Q_{E} and Q_{M} are set to zero (Q_{E} = Q_{M} = 0), the matrices A and D for a non-magnetic ENG and MNG medium is obtained.
We are going to investigate the influence of polar magnetization on spectrum responses of the single layer of the bi-gyrotropic ENG and MNG materials and finally multilayer structures (MPCs) which include bi-gyrotropic single- negative magnetic materials.
In our previous work [19] we indicated that the performances of both bi- gyrotropic ENG and MNG layers in presence of longitudinal magnetization were pretty similar together. The results have revealed a nearly perfect reflectance for all values, and a larger Kerr rotation for the bi-gyrotropic ENG layer was obtained rather than MNG one. If we want to compare such situation in presence of polar magnetization, we will find giant Kerr rotations rather than longitudinal magnetization case. In polar geometry, both reflectance and Kerr rotation parameters have larger amounts for a single ENG layer rather than MNG one.
Figures 1 and 2 show the numerical results for both bi-gyrotropic (a) ENG and (b) MNG magnetic media, respectively. In Fig. 1, the reflectance and Kerr rotation of a half-wave bi-gyrotropic (a) ENG layer (with ε_{1} = −3 and μ_{1} = 3) and (b) MNG layer (with ε_{1} = 3 and μ_{1} = −3) as functions of non-diagonal components (ε_{2} and μ_{2} ) have been illustrated; while Fig. 2 shows such optical and magneto-optical parameters as functions of diagonal components (ε_{1} and μ_{1} ) for (a) ENG and (b) MNG magnetic media with ε_{2} = μ_{2} = 0.1 (according to optimal responses in Fig.1). In both figures, the numerical computations have been done for the case of normal incidence of light at wavelength of 1550 nm and in presence of polar magnetization. The results show that, in presence of polar magnetization, the performance of bi- gyrotropic ENG layer is more significant rather than bigyrotropic MNG layer, too.
The focus of present research has been on the potential of using polar bi- gyrotropic single-negative magnetic materials to act simultaneously as reflector and magneto-optical rotator. Accordingly, we have firstly employed a 4×4 the transfer matrix method to understand the interaction between an electromagnetic field and such magnetic metamaterials. we have numerically demonstrated that a single layer of polar bi-gyrotropic ENG or MNG magnetic material can show notable reflectance and Kerr rotation, simultaneously, and can significantly enhance the operation of multilayer structures.
1. | A. Alu, N. Enghetal, A. Erentok, R.W. Ziolkowski, Single-Negative, Double-Negative, and Low-index Metamaterials and their Electromagnetic Applications IEEE Transact. Anten. Propag. Mag. 49 (2007) 23-36. |
2. | D.L. Vu, V.T. Pham, T.V. Do, T.T. Nguyen, T.T.T. Vu, V.H. Le, Y.P. Lee, The electromagnetic response of different metamaterial structures, Adv. Nat. Sci: Nanosci. Nanotechnol. 1 (2010) 045016. |
3. | K. B. Thapa, A. Vishwakarma, R. Singh, S. P. Ojha, Electromagnetic Wave Propagation Through Single Negative, J. Ovon. Res. 6 (2010) 105–115. |
4. | H.X. Xu, G.M. Wang, M.Q. Qi, H.Y. Zeng, Ultra-small single- negative electric metamaterials for electromagnetic coupling reduction of microstrip antenna array, Opt. Express 20 (2012) 21968-21976. |
5. | J.B. Pendry, Negative Refraction Makes a Perfect Lens, Phys. Rev. Lett. 85 (2000) 3966-3969. |
6. | W.F. Michael, S.K. Yuri, Sub-wavelength imaging with a left- handed material flat lens, Phys. Lett. A 334 (2005) 324-330. |
7. | T. Tang, Trapping of electromagnetic wave in single-negative metamaterial waveguides, Optik 124 (2013) 6242– 6244. |
8. | T. Tang, F. Chen, B. Sun, Tunneling modes in photonic crystals with anisotropic single-negative metamaterials, Opt. Las. Technol. 43 (2011) 237-241. |
9. | T. Tang, W. Liu, X. Gao, X. He, J. Yang, Band gaps and nonlinear defect modes in one-dimensional photonic crystals with anisotropic single-negative metamaterials, Opt. Las. Technol. 43 (2011) 1016-1019. |
10. | R. Zeng, Y. Yang, Sh. Zhu, Casimir force between anisotropic single-negative metamaterials, Phys. Rev. A 87 (2013) 063823. |
11. | M.S. Rill, C.E. Kriegler, M. Thiel, G.V. Freymann, S. Linden, M. Wegener, Negative-index bianisotropic photonic metamaterial fabricated by direct laser writing and silver shadow evaporation, Opt. Lett. 34 (2009) 19-21. |
12. | C.E. Kriegler, M.S. Rill, S. Linden, M. Wegener, Bianisotropic Photonic Metamaterials, IEEE J. Select. Top. Quant. Electron. 16 (2010) 367-375. |
13. | T.G. Mackay, A. Lakhtakia, Negative refraction, negative phase velocity, and counterposition in bianisotropic materials and metamaterials, Phys, Rev. E 79 (2009) 026610. |
14. | A.G. Gurevich, G.A. Melkov, Magnetization oscillation and Waves (CRC Press Inc., New York, 1996). |
15. | A.K. Zvezdin, V.A. Kotov, Modern Magnetooptics and Magnetooptical Materials (Bristol and Philadelphia: Institute of Physics Publishing, 1997). |
15. | A.K. Zvezdin, V.A. Kotov, Modern Magnetooptics and Magnetooptical Materials (Bristol and Philadelphia: Institute of Physics Publishing, 1997). |
16. | J. Zak, E.R. Moog, C. Liu, S.D. Bader, J. Magn. Magn. Mater. 89 (1990) 107. |
17. | M. Zamani, H. Nezhad Hajesmaeili, M.H. Zandi, Opt. Mater. 58 (2016) 38-45. |
18. | . Zamani, H. Nezhad Hajesmaeili, M.H. Zandi, J. Phys. Condens. Matter 29 (2017) 035901. |
19. | H. Nezhad Hajesmaeili, M. Zamani, M.H. Zandi, Photonics. Nanostruct. Fundam. Appl. 24 (2017) 69-75. |
20. | M. Zamani. S. Eftekhari, M. Ghanaatshoar, Universal approach for appending double-negative materials to magneto-optics in multilayer structures, Mater. Res. Express 5 (2018) 046102. |
17. | M. Zamani, H. Nezhad Hajesmaeili, M.H. Zandi, Opt. Mater. 58 (2016) 38-45. |
18. | M. Zamani, H. Nezhad Hajesmaeili, M.H. Zandi, J. Phys. Condens. Matter 29 (2017) 035901. |
19. | H. Nezhad Hajesmaeili, M. Zamani, M.H. Zandi, Photonics. Nanostruct. Fundam. Appl. 24 (2017) 69-75. |
© 2018 Hamidreza Nezhad Hajesmaeili et al.; licensee Payam Publishing Pvt. Lt..
This is an Open Access article under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The license is subject to the Magnetic Materials Advances terms and conditions: (http://www.jfips.com/saea)